text: While the above techniques use a spatially extended, wide incident beam, section topography is based on a narrow beam on the order of some 10 micrometers (in one or, in the case of pinhole topography with a pencil beam, in both lateral dimensions). Section topographs therefore investigate only a restricted volume of the sample.
  On its path through the crystal, the beam is diffracted at different depths, each one contributing to image formation on a different location on the detector (film). Section topography can therefore be used for depth-resolved defect analysis.
  In section topography, even perfect crystals display fringes. The technique is very sensitive to crystalline defects and strain, as these distort the fringe pattern in the topograph. Quantitative analysis can be performed with the help of image simulation by computer algorithms, usually based on the Takagi-Taupin equations.
  An enlarged synchrotron X-ray transmission section topograph on the right shows a diffraction image of the section of a sample having a gallium nitride (GaN) layer grown by metal-organic vapour phase epitaxy on sapphire wafer. Both the epitaxial GaN layer and the sapphire substrate show numerous defects. The GaN layer actually consists of about 20 micrometers wide small-angle grains connected to each other. Strain in the epitaxial layer and substrate is visible as elongated streaks parallel to the diffraction vector direction. The defects on the underside of the sapphire wafer section image are surface defects on the unpolished backside of the sapphire wafer. Between the sapphire and GaN the defects are interfacial defects.